Application code AS1554.1-2004 Material 1 Low carbon steel Welding process MMAW Material 2 Joint type Fillet weld Thickness 12 mm Position 3F Diameter N/A Thermal conditions Welding technique/Preparation Min preheat Nil above 10 °C Preparation method Machine, flame cut and/or grind Method Flame (propane) if required Gouge method N/A Temp. check Digital or temp. crayons Interpass cleaning Grind and/or wire brush Arc energy Max bead MMAW-4 x electrode diameter Max interpass temp. Electrical out N/A PWHT None Shielding gas flow N/A gas flow N/A Ref Consumable brand Consumable classification Consumable treatment A E4113 Stored dry Weld details Electrode/ Flux Welding parameters Travel speed Filler Pass Process Side Pos Dir Ref Size Or Gas Pol Amps Volts (mm/min) 1 MMAW 1 3F A 3.2 AC 120 22 90 2 MMAW 1 3F A 3.2 AC 115 22 100 Notes 1. Visual inspection to comply with AS1554.1:2004 GP Category Table 6.2. Approved Approved client Release stamp
Application code Welding process Joint type Position AS1554.1-2004 MMAW Fillet weld 3F Material 1 Material 2 Thickness Diameter Low carbon steel 12 mm N/A Thermal conditions Welding technique/Preparation Min preheat Method Temp. check Arc energy Max interpass temp. PWHT Nil above 10 °C Flame (propane) if required Digital or temp. crayons None Preparation method Gouge method Interpass cleaning Max bead Electrical out Shielding gas flow gas flow Machine, flame cut and/or grind N/A Grind and/or wire brush MMAW-4 x electrode diameter N/A N/A N/A Ref Consumable brand Consumable classification Consumable treatment A E4113 Stored dry Weld details Electrode/ Filler Flux Welding parameters Travel speed Pass Process Side Pos Dir Ref Size Or Gas Pol Amps Volts (mm/min) 1 2 MMAW MMAW 1 1 3F 3F A A 3.2 3.2 AC AC 120 115 22 22 90 100 Notes 1. Visual inspection to comply with AS1554.1:2004 GP Category Table 6.2. Approved Approved client Release stamp